Water Droplet Erosion Resistant Materials and Surface
Mohammad Sadegh Mahdipoor
In the Department
Mechanical and Industrial Engineering
Presented in Partial Fulfillment of the Requirements
For the Degree of Doctor of Philosophy (Mechanical and Industrial Engineering) at
Montreal, Quebec, Canada
SCHOOL OF GRADUATE STUDIES
This is to certify that the thesis prepared
By: Mohammad Sadegh Mahdipoor
Entitled: Water droplet erosion resistant materials and surface treatments
and submitted in partial fulfillment of the requirements for the degree of Doctor of Philosophy (Mechanical Engineering)
Complies with the regulations of the University and meets the accepted standards with respect to originality and quality.
Signed by final examining committee:
_____________________________________________Chair Dr. Amr Youssef _____________________________________________External Examiner Dr. Mohammad Jahazi ______________________________________________External to Program Dr. Michelle Nokken ______________________________________________Examiner Dr. Martin Pugh _______________________________________________Examiner Dr. Ramin Sedaghati _______________________________________________Thesis Supervisor Dr. Mamoun Medraj Approved by: ________________________________________________________ Chair of Department or Graduate Program Director
Water Droplet Erosion Resistant Materials and Surface Treatments
Mohammad Sadegh Mahdipoor Concordia University, 2016
Water Droplet Erosion (WDE) is a mechanical degradation which is of great concern to power generation and aerospace industries, where water droplets interact with high-speed moving components. It is observed on multiple components of airplanes when flying in the rain, on steam turbine blades, and gas turbine compressor blades which is the focus of this study. Compressor blades in gas turbines suffer from WDE due to the recently implemented technology Inlet Fog Cooling. It is utilized to boost gas turbine efficiency in high ambient temperatures via the spraying of micro-sized water droplets into the intake air. Evaporation of water droplets cools the intake charge and increases the air density. The main drawback of inlet cooling is that part of the water droplets are carried into the compressor by intake air flow, which is called overspray. Repetitive impact between rotating blades and water droplets leads to WDE damage, which is a major problem.
This study attempted to improve WDE resistance of compressor blades made of Ti6Al4V. Two different approaches were considered: Studying WDE of TiAl alloy as a potential erosion resistant material for turbine blades and Surface engineering of Ti6Al4V via gas nitriding and HVOF spraying of WC-Co. To investigate WDE in this work, erosion experiments were carried out using the state-of-art WDE rig available at Thermodynamics of Materials Group (TMG), Concordia University. It enables control of erosion conditions such as impact velocity, impact angle, droplet size, and droplet impingement number.
In the first stage of this study, WDE of nearly fully lamellar TiAl alloy was directly compared to Ti6Al4V at relatively wide ranges of impact speed (i.e. 275m/s, 300m/s, 325m/s and 350m/s) and droplet size (i.e. 464µm and 603µm). TiAl demonstrated superior erosion performance (i.e. longer incubation period and slower material loss) compared with Ti6Al4V at all tested conditions. Herein, the relation of impact velocity and maximum erosion rates for TiAl and Ti6Al4V alloys was established and the damage threshold speeds of TiAl were determined. Afterwards, the erosion behaviour of TiAl was related to its mechanical properties and irregular
microstructure. Lastly, in-depth investigation was carried out to reveal erosion damage mechanism of TiAl at different stages including incubation, material loss initiation, maximum erosion rate, and advanced stages.
In the second stage of this study, the influence of gas nitriding on water droplet erosion behaviour of Ti6Al4V was investigated. Ti6Al4V coupons were nitrided at two different temperatures (i.e. 900 and 1050°C) for 5 and 10 hours and the nitrided coupons were characterized. Their erosion behaviour in comparison with as-received and annealed Ti6Al4V was examined at two impact speeds (i.e. 300m/s and 350m/s). Mechanical properties, erosion performance and damage mechanism of treated Ti6Al4V were significantly influenced by the nitriding temperature. Exploring the potential of HVOF spray WC-Co coating to combat WDE was the last part of this study. Erosion performance of two WC-Co coatings was examined at 250m/s, 300m/s and 350m/s impact speeds in comparison with Ti6Al4V. The as-sprayed coating did not show notable WDE protection; however, removing its top layers and smoothing its surface notably improved the erosion performance.
To my loving parents, Pari Azizi and Saleh Mahdipoor And to my little but supportive sister, Mahshid
Who always help me to find my Smile Without them I would never have finished this work
This research would not have been possible without constant guidance, support and advice of my supervisor, Professor Mamoun Medraj. He gave me a passion to learn more, freedom to find my path and instruction to stay in the right track. I am sincerely grateful to have this opportunity working under his supervision at TMG group, where I learned so many things.
I would like to thank Dr. Mohammad Jahazi, Dr. Michelle Nokken, Dr. Martin Pugh and Dr. Ali Dolatabadi for serving on my committee and providing guidance toward the completion of this degree.
I wish to thank Dr. Christian Moreau, Dr. Ali Dolatabadi, Dr. Martin Pugh, and Dr. Robin Drew for giving me permission to use the facilities in their laboratories. I am grateful to Dr. Dmytro Kevorkov and Dr. Pawel Jedrzejowski for their insightful comments and contributions in this work. I also like to thank Mr. Mazen Samara, who was always patient and helpful in the laboratories. Very warm thanks to all TMG members especially to: Hany Kirols, Dr. Ahmad Omar Mostafa, Jessie Yi, Guy Joel Rocher, Tian Wang, Benjamin Wallace, Bolarinwa Komolafe, Alex Chen, and Dina Ma. Thank you for the help with the experiments, the constructive discussions and the valuable suggestions. I wish to extend my thanks to Dr. Niloofar Kamkar from Ecole Technologie Superieure (ETS) for all the great helps during my PhD. I would like to also thank Dr. Fadhel Ben Ettouil, Dr. Fariba Tarasi and Dr. Samir Mourad for their helps through the experiments in Concordia and ETS Universities. I wish you all success in your endeavours.
This work was financially supported by Rolls-Royce Canada Ltd., the Consortium for Research and Innovation in Aerospace in Quebec (CRIAQ) under CRIAQ-MANU419 project and Natural Sciences and Engineering Research Council of Canada (NSERC). The financial support is acknowledged.
Friends, I wish to thank my amazing friends who were always there for me throughout the most challenging moments. My heartfelt thank goes to my lovely sister and wonderful friend, Mahshid, who always makes me smile regardless how much it was difficult time. I give my deepest appreciation to my uncles, Reza and Bahram, for their endless support, care and encouragement.
Though no amount of “Thank You” will suffice, I would like to wholeheartedly thank my parents, Pari and Saleh who are the foundation of my life. I am thankful for your boundless support
and unconditional love throughout my entire life. You have always inspired me to be a better person. Every day I have learned new things just by watching you. Watching and learning the real compassion, devotion and dedication. Without each of you, I would be nowhere near the person I am. Thank You.
Table of Contents
List of figures ... xii
List of tables ... xviii
Chapter 1 : Introduction ... 1
1.1. Water droplet erosion ... 1
1.1.1. Physics of the water droplet impact on a solid surface ... 3
1.1.2. Damage mechanism of water droplet erosion ... 6
22.214.171.124. Early stages of erosion ... 7
126.96.36.199. Advanced stages of erosion and material removal ... 9
1.1.3. Parameters affecting liquid droplet erosion ... 11
188.8.131.52. Impact speed ... 11
184.108.40.206. Impact angle ... 11
220.127.116.11. Droplet size ... 12
1.1.4. Time dependence of water droplet erosion ... 13
1.1.5. Representation of water droplet erosion results ... 14
1.2. Promising water droplet erosion resistant materials and surface treatments... 17
1.3. Objectives ... 21
1.4. Thesis layout ... 22
Chapter 2 : Influence of impact speed on water droplet erosion of TiAl compared with Ti6Al4V ... 24
ABSTRACT ... 24
2.1. Introduction and literature review ... 25
2.2. Materials and experimental procedures ... 30
2.2.1. Materials ... 30
2.2.2. Water droplet erosion test ... 31
2.2.3. Imaging techniques ... 35
2.3. Results ... 35
2.3.1. Surface hardness and roughness of erosion test coupons ... 35
2.3.2. Droplet size distributions ... 36
2.3.3. Water droplet erosion performance of TiAl and Ti6Al4V alloys ... 37
18.104.22.168. Cumulative erosion, incubation period and maximum erosion rate ... 37
22.214.171.124. Influence of impact speed on incubation period and erosion rate ... 39
126.96.36.199. Comparison between TiAl and Ti6Al4V WDE performances ... 43
188.8.131.52. Microscopic observation of erosion damage ... 45
2.4. Discussion ... 47
2.5. Conclusions ... 52
Relating to the theme of thesis ... 53
Chapter 3 : Water droplet erosion mechanism of nearly fully-lamellar gamma TiAl alloy ... 54
ABSTRACT ... 54
3.1. Introduction and literature review ... 55
3.2. Material and experimental procedure... 57
3.2.1. Material and preparation ... 57
3.2.2. Water droplet erosion experiments ... 58
3.2.3. Damage analysis ... 59
3.3. Results and discussion ... 59
3.3.1. Systematic analysis of erosion damage at different stages ... 59
184.108.40.206. Incubation stage: microscopic observation ... 59
220.127.116.11. Maximum erosion rate stage ... 65
18.104.22.168.1. Microscopic observation of eroded TiAl once material loss starts ... 65
22.214.171.124.2. Microscopic observation of eroded TiAl at maximum erosion rate stage ... 67
126.96.36.199. Terminal stage ... 68
188.8.131.52.1. Characterization of erosion craters and damage progress ... 68
184.108.40.206.1.2. Damage progress on the sidewalls of erosion crater ... 70
3.3.2. Micro-analysis and fractographic interpretation of eroded TiAl at terminal stage ... 70
3.4. Proposed water droplet erosion mechanism for nearly fully lamellar TiAl alloy ... 76
3.5. Conclusions ... 80
Relating to the theme of thesis ... 81
Chapter 4 : Water droplet erosion behavior of gas nitrided Ti6Al4V ... 82
ABSTRACT ... 82
4.1. Introduction and literature review ... 83
4.2. Material and experimental procedures ... 85
4.2.1. Material ... 85
4.2.2. Gas nitriding treatment ... 85
4.2.3. Characterization of nitrided specimens ... 86
4.2.4. Water droplet erosion test ... 87
4.3. Results and discussion ... 89
4.3.1. Microstructural investigation ... 89
4.3.2. Microhardness of nitrided specimens... 94
4.3.3. Water droplet erosion ... 97
220.127.116.11. Water droplet erosion performance ... 97
18.104.22.168.1. Water droplet erosion performance at impact speed of 350m/s ... 98
22.214.171.124.2. Water droplet erosion performance at impact speed of 300m/s ... 100
126.96.36.199.3. Influence of nitriding atmosphere on the erosion performance ... 102
188.8.131.52.4. Cumulative erosion resistance ... 103
184.108.40.206. Characterization of erosion damage ... 105
4.4. Conclusions ... 110
Relating to the theme of thesis ... 112
Chapter 5 : HVOF sprayed coatings of nano-agglomerated tungsten-carbide/cobalt powders for water droplet erosion application ... 113
ABSTRACT ... 113
5.1. Introduction and literature review ... 114
5.2. Materials and experimental procedure ... 117
5.2.1. Materials ... 117
5.2.2. HVOF coating process ... 117
5.2.3. Coating characterization ... 118
5.2.4. Water droplet erosion test ... 118
5.3. Results ... 120
5.3.1. As-sprayed coatings characterization ... 120
5.3.2. Water droplet erosion results ... 122
5.3.3. Microstructural characteristics of eroded coatings ... 125
5.4. Discussion ... 128
5.4.1. Water droplet erosion damage at different impact speeds ... 128
5.4.2. Erosion mechanism of spray coatings ... 130
5.5. Conclusions ... 133
Relating to the theme of thesis ... 135
Chapter 6 : Concluding remarks ... 136
6.1. Conclusions ... 137
6.2. Contributions ... 140
6.3. Recommendations for future works ... 142
References ... 144
Appendices ... 156
Appendix A ... 156
A.1. Water droplet erosion rig ... 156
A.2. Measurement of droplet sizes and plotting their size distribution ... 157
A.3. Pattern of impacting droplets in each rotation ... 158
List of figures
Figure 1-1: (a) Schematic of water droplet formation in the steam turbines , (b) severe water droplet
erosion on suction side of steam turbine blades  ... 2
Figure 1-2: (a) Schematic of a gas turbine equipped with fog cooling system , (b)eroded blade of HP compressor in LM6000 turbine  ... 2
Figure 1-3: Schematic presentation of a water droplet impingement onto a solid surface: (a) upon impact and before the detachment of disturbed region, (b) after the detachment of disturbed region [3, 23] ... 4
Figure 1-4: Schematic presentation of: (a) stress waves travelling in the target, (b) reflection and interference of longitudinal and Rayleigh waves [16, 18] ... 5
Figure 1-5: Schematic of erosion damage initiation on a ductile solid surface proposed by Field et al.  ... 7
Figure 1-6: Eroded surface of: (a) polymethyl methacrylate showing ring fractures , (b) zinc sulphide showing an undamaged area surrounded by annular fractures , (c) aluminum showing the rim of depression and the revealed grain boundaries  ... 9
Figure 1-7: Normalized material loss of stainless steel eroded at different impact angles  ... 12
Figure 1-8: Different forms of erosion graphs  ... 13
Figure 1-9: (a) Typical water droplet erosion and (b) erosion rate graphs showing five different stages  ... 14
Figure 1-10: (a) Typical S-shaped erosion graph plotted through experimental points, (b) extracting the erosion indicators from material loss graphs [2, 54] ... 16
Figure 1-11: Different surface treatments of titanium alloys: (a) thermal treatments, (b) thermochemical treatments, (c) thin film deposition, (d) thermal spray coating ... 18
Figure 1-12: Cumulative erosion resistance of TiAl intermetallic and surface treated Ti6Al4V normalized to that of reference material [48, 61, 67, 68, 74-76, 78-81] ... 20
Figure 1-13: Flowchart of the thesis ... 23
Figure 2-1: SEM micrographs of: (a) annealed Ti6Al4V, (b) HIP TiAl... 31
Figure 2-2: Schematic of the water droplet erosion rig and droplet size measuring setup ... 32
Figure 2-3: Erosion results of three Ti6Al4V coupons tested at 350m/s impact speed and 464µm droplet size showing repeatable experimental results ... 35
Figure 2-4: The number and volume droplet size distributions of 200 droplets generated using nozzle 1. 36
Figure 2-5: The number and volume droplet size distributions of 200 droplets generated using nozzle 2. 36
Figure 2-6: Water droplet erosion results, material loss versus volume of impinging water, for Ti6Al4V specimens tested at different impact speeds and droplet size of (a) 464µm, (b) 603µm ... 37
Figure 2-7: Water droplet erosion results, material loss versus volume of impinging water, for TiAl specimens tested at different impact speeds and droplet size of (a) 464µm, (b) 603µm ... 38
Figure 2-8: Maximum erosion rate of Ti6Al4V and TiAl alloys eroded by 464 and 603μm water droplets at four different impact speeds ... 38
Figure 2-9: Incubation period of Ti6Al4V and TiAl alloys eroded by 464 and 603μm water droplets at four different impact speeds ... 39
Figure 2-10: The dependency of Ti6Al4V and TiAl incubation period on the impact speeds when they are eroded by 464µm water droplets. The arrow indicates the test performed at 250m/s caused no measurable erosion after 106 impacts ... 41
Figure 2-11: The dependency of Ti6Al4V and TiAl incubation period on the impact speeds when they are eroded by 603µm water droplets. The arrow indicates the test performed at 200m/s caused no measurable erosion after 106 impacts ... 42
Figure 2-12: Dependency of maximum erosion rate on the impact speed for Ti6Al4V and TiAl alloys eroded by 464μm water droplets ... 42
Figure 2-13: Dependency of maximum erosion rate on the impact speed for Ti6Al4V and TiAl alloys eroded by 603μm water droplets ... 43
Figure 2-14: Material loss superiority of TiAl compared to Ti6Al4V during the WDE test performed using 464μm drops ... 44
Figure 2-15: Material loss superiority of TiAl compared to Ti6Al4V during the WDE test performed using 603µm drops ... 45
Figure 2-16: Micrographs of erosion craters at different time intervals (mentioned between two images) for the erosion experiments performed at 325m/s impact speeds and 603µm droplet size: (a) Ti6Al4V, (b) TiAl ... 46
Figure 2-17: Cross sectional SEM micrographs of eroded (a and b) Ti6Al4V and (c and d) TiAl: (a and c) erosion pits at early stages, (b and d) edges of erosion crater showing the influence of local microstructure on cracking behavior ... 46
Figure 2-18: Surface hardness of TiAl and Ti6Al4V presented in 0.5min intervals during the incubation of erosion experiment performed at 350m/s using 464µm droplets ... 48
Figure 3-1: SEM micrographs of TiAl alloy: (a) low magnification showing the random oriented colonies, (b) high magnification showing the lamellar microstructure ... 57
Figure 3-2: (a) WDE result (cumulative material loss) of TiAl and the appearance of erosion line at different stages : (1) incubation stage, (2) maximum erosion rate stage, (3) terminal steady state stage, (b) Schematic of water droplet erosion investigation ... 59
Figure 3-3: SEM micrographs of slightly eroded TiAl at incubation period showing: (a) localized material flow, (b) different responses of colonies to droplet impacts, (c) slip bands impeded by colony boundaries, (d) micro-twinning within the γ layers ... 61
Figure 3-4: Schematic of different orientation of the colonies subjected to water droplet impacts ... 62
Figure 3-5: AFM images of: (a) original polished surface of TiAl (b) eroded surface of TiAl after 100,000 droplet impacts ... 63
Figure 3-6: (a) AFM height image of a deformed colony and extracted average height profiles along two lines, (b) SEM micrograph of another deformed colony showing two lines with similar conditions ... 64
Figure 3-7: (a) SEM micrograph of eroded surface showing interlamlellar cracks nucleation, (b) SEM micrograph of eroded surface showing interlamellar cracking near colony boundaries, (c) cross sectional SEM micrograph of slightly eroded surface showing a sub-surface crack ... 65
Figure 3-8: SEM micrograph from eroded surface of TiAl after 400,000 droplet impacts, demonstrating severe local plastic deformation, micro-cracking and micro-pitting... 66
Figure 3-9: SEM micrograph of an isolated erosion crater forming during the maximum erosion rate stage ... 68
Figure 3-10: Cross sectional SEM micrographs of isolated erosion craters showing hydraulic penetration at: (a) Early stage, (b) evolved stage, leading to formation of an undercutting pit ... 68
Figure 3-11: (a) SEM micrograph of complete erosion damage line, (b) cross section of eroded TiAl showing wide and shallow pit with relatively smooth surface, (c) cross section of eroded TiAl showing a jagged surface, (d) cross section of eroded TiAl showing formation of an undercutting void at the bottom of crater, (e) cross section of eroded TiAl showing sever damage ... 70
Figure 3-12: SEM micrographs from cross sections of eroded TiAl at terminal stage of erosion,
Figure 3-13: Distribution of different types of cracks observed on the edges of erosion craters ... 73
Figure 3-14: Length distribution of different types of cracks observed on the edges of erosion craters .... 75
Figure 3-15: SEM micrographs of eroded TiAl at terminal stage of erosion: (a) fracture surface evolved by intergranullar cracks, (b) cross sectional view showing intergranullar cracks... 75
Figure 3-16: SEM micrographs from the surface of eroded TiAl at terminal stage (inside the erosion craters): (a) translamellar fracture surface, (b) interlamellar fracture surface and mixed fracture surface . 76 Figure 3-17: Schematic of: (a) extrusion/intrusion pattern and potential sites for cracks nucleation , (b) high speed strike of lateral jets to the exaggerated extrusion and subsequent cracks initiation  ... 78
Figure 4-1: BSE-SEM micrographs of as-received Ti6Al4V ... 85
Figure 4-2: Different steps of nitriding process ... 86
Figure 4-3: Schematic of the water droplet erosion rig ... 89
Figure 4-4: Appearance of as-received Ti6Al4V and nitrided Ti6Al4V coupons ... 90
Figure 4-5: XRD patterns of as-received Ti6Al4V and nitrided coupons ... 91
Figure 4-6: SE-SEM micrographs of the surface of nitrided Ti6Al4V: (a) 900C-5h, (b) 1050C-5h ... 91
Figure 4-7: (a) OM and (b,c) BSE-SEM cross sectional micrographs of Ti6Al4V nitrided at 900 ̊C for 5 hours ... 94
Figure 4-8: (a) OM and (b) BSE-SEM cross sectional micrographs of Ti6Al4V nitrided at 1050 ̊C for 5 hours ... 94
Figure 4-9: Microhardness profiles of nitrided Ti6Al4V at 900 ̊C ... 97
Figure 4-10: Microhardness profiles of nitrided Ti6Al4V at 1050 ̊C ... 97
Figure 4-11: WDE results of the samples treated at 900°C using impact speed of 350m/s: (a) normalized material loss versus volume of impinging water, (b) the instantaneous erosion rate at different intervals 99 Figure 4-12: WDE results of the samples treated at 1050°C using impact speed of 350m/s: (a) normalized material loss versus volume of impinging water, (b) the instantaneous erosion rate at different intervals ... 100
Figure 4-13: WDE results of the samples treated at 900°C using impact speed of 300m/s: (a) normalized material loss versus volume of impinging water, (b) the instantaneous erosion rate at different intervals ... 101
Figure 4-14: WDE results of the samples treated at 1050°C using impact speed of 300m/s: (a) normalized material loss versus volume of impinging water, (b) the instantaneous erosion rate at different intervals ... 102
Figure 4-15: Water droplet erosion results of nitrided Ti6Al4V at N2 and N2-4%H2 environments using
impact speed of 350m/s: (a) erosion graph, (b) material loss superiority of nitrided Ti6Al4V compared to Ti6Al4V during the WDE test ... 103
Figure 4-16: Water droplet erosion results of nitrided Ti6Al4V at N2 and N2-4%H2 environments using
impact speed of 300m/s: (a) erosion graph, (b) material loss superiority of nitrided Ti6Al4V compared to Ti6Al4V during the WDE test ... 103
Figure 4-17: Optical micrographs of erosion craters at different time intervals of the erosion experiments carried out at 300m/s impact speed: (a) 900C-5h, (b) 1050C-5h, (c) H-900C-5h, (d) as-received Ti6Al4V ... 106
Figure 4-18: Surface BSE-SEM micrographs of nitrided Ti6Al4V (900C-5h) after erosion test: (a) erosion crater and deep pitting, (b) damage initiation on the compound layer, (c) top layers detachment at the edge of erosion crater, (d) erosion damage on diffusion layer, (e) eroded surface inside the erosion crater .... 108
Figure 4-19: (a) Surface BSE-SEM micrograph of slightly eroded 1050C-5h sample, (b) cross section of 1050C-5h sample (non-eroded) showing diffusion layer ... 108
Figure 4-20: Cross sectional BSE-SEM micrographs of nitrided Ti6Al4V at 900°C after erosion test showing: (a) erosion damage of nitrided layers, (b) main erosion crater at low magnifications, (c) cracks propagation and hydraulic penetration ... 110
Figure 4-21: Cross sectional BSE-SEM micrographs of nitrided Ti6Al4V at 1050°C after erosion test showing: (a) erosion damage of nitrided layers, (b) main erosion crater at low magnifications, (c) cracks propagation and hydraulic penetration ... 110
Figure 5-1: Schematic of the water droplet erosion rig ... 119
Figure 5-2: XRD patterns of (a) Sulzer 5810 powder and SP coating, (b) Woka 3110 powder and SD coating ... 121
Figure 5-3: SEM micrographs showing cross sections of as-sprayed: (a) SP coating at low magnification, (b) SP coating at high magnification, (c) SD coating at low magnification, (d) SD coating at high
magnification ... 122
Figure 5-4: Cumulative volume loss per unit area vs. cumulative volume of water impacting unit area at the impingement speed of 250m/s ... 124
Figure 5-5: Cumulative volume loss per unit area vs. cumulative volume of water impacting unit area at the impingement speed of 300m/s ... 124
Figure 5-6: Cumulative volume loss per unit area vs. cumulative volume of water impacting unit area at the impingement speed of 350m/s ... 124
Figure 5-7: Cross sectional SEM images showing the depth and texture of the erosion craters at impact speed of 250m/s: (a) SP coating, (b) SD coating ... 125
Figure 5-8: Cross sectional SEM images of eroded SP coating along the edges of erosion crater, WDE conditions: 464μm droplet size and 300m/s impact speed ... 126
Figure 5-9: Cross sectional SEM images of eroded SD coating along the edges of erosion crater, erosion conditions: 464μm droplet size, 300m/s impact speed ... 128
Figure 5-10: Schematic of water impact on a cermet coating with its typical splat microstructure: (a) as-sprayed cermet coating before water impact, (b) upon impact and formation of water jet, (c) Eroded cermet coating exposed to water droplet impingement in advanced ... 133
Figure 6-1: Normalized cumulative erosion resistance of all tested coupons at 300m/s ... 136
List of tables
Table 2-1: The impact speed exponent in Equation 1-1 found in different water erosion investigations ... 27
Table 2-2: Mechanical properties of Ti6Al4V and TiAl* [69, 86, 88-91]... 31
Table 2-3: Impact pressure and time duration of one impact pulse calculated for different erosion conditions based on Equations 2-9 and 2-10 ... 40
Table 4-1: Nitriding conditions of Ti6Al4V ... 86
Table 4-2: Microhardness and erosion performance of as-received, annealed and nitrided Ti6Al4V ... 104
Table 5-1: Chemical composition of the feedstock used in the experiments ... 117
Table 5-2: The characteristics of as-sprayed coatings ... 122
Table 5-3: Maximum erosion rate (ERmax) and cumulative erosion resistance (CER) of the coatings and Ti6Al4V ... 125
1.1. Water droplet erosion
The word "erosion" is derived from the word “rodere”, which is a Latin verb and means “gnaw”. This word is widely used to describe wearing of rocks, sea shores, and soil by water and wind; however, in material science it is used to describe a mechanical damage caused by high speed impingements . Erosion is the result of either solid/solid or liquid/solid interactions. Different types of erosion are known such as solid particle erosion, cavitation erosion, liquid impingement erosion, and slurry erosion. They are all associated with the cyclic loading and sharp pressure pulses [2-4]. Compared to solid particle erosion and cavitation erosion, liquid impingement erosion has not been well studied.
In the field of aerospace and power generation, water droplet erosion (WDE) refers to a progressive material loss caused by repetitive high speed impact of water droplets [2, 5]. WDE is a sub-category of liquid impingement erosion. It is widely observed in turbine blades, aircraft aerofoils, missiles, helicopter rotors, and the inner wall of certain steam pipes . Also, it is a well-known damage for steam turbine blades, shown in Figure 1-1, and scientists have attempted to address this phenomenon since the beginning of 20th century [6, 7]. When steam reaches to the last stages of turbine, because of low pressure and temperature small portion of steam goes below the saturation line and causes the formation of very small primary water droplets, which is called fog droplets. Such droplets coalesce and form a water film on the stationary blades. Accumulation of more water makes the water film unstable and leads to the formation of large droplets (more than 1mm). The large droplets are atomized and then brought with the steam flow to the plane of rotating blades . The schematic of water droplet formation in steam turbines is demonstrated in Figure 1-1-a. The supersonic impingement of rotating blades and generated water droplets cause WDE, as shown in Figure 1-1-b. This type of erosion has also been observed on the blades of gas turbine compressor when fog cooling system is used [5, 9], shown in Figure 1-2. It is known that turbine efficiency decreases 0.3-0.5% by raising 1°F ambient temperature . Fog cooling, spraying small water droplets to cool the intake air, is introduced as a practical approach to enhance the turbine efficiency through increasing air density. During fog cooling the sprayed water droplets partially evaporate; however, some of them remain and enter the compressor with the intake air, called overspray [5, 9, 11]. Successive high speed impingements between these droplets and
rotating blades result in water droplet erosion damage on their leading edge. This damage leads to material loss, distortion of the blades profile, and reduction of their aerodynamic performance. Moreover, weight loss of the blades may influence the balance of compressor and cause significant vibrations, which is a major issue for the engine.Hence, understanding water droplet erosion and reducing this damage is of high interest for power generation industries.
Figure 1-1: (a) Schematic of water droplet formation in the steam turbines , (b) severe water droplet erosion on suction side of steam turbine blades 
Figure 1-2: (a) Schematic of a gas turbine equipped with fog cooling system , (b)eroded blade of HP compressor in LM6000 turbine 
1.1.1. Physics of the water droplet impact on a solid surface
To explain the WDE, first the physics of a single liquid/solid impingement are reviewed. Upon impingement of single droplet onto a solid surface pressure pulses are generated and form a disturbed zone (shocked envelop) inside the liquid, close to liquid/solid interface , shown in Figure 1-3-a. After a few micro seconds, the compressed region of liquid breaks away. This moment, which is followed by the formation of lateral outflow jets, is commonly referred to as “stagnation moment”. The generated jets travel across the surface with velocities up to 10 times the impact speed [3, 16, 19]. They are detrimental and play a notable role in initiating the erosion damage [2, 3, 20]. Once the disturbed region of water breaks away, the potential energy of compressed water transforms to kinetic and the impact pressure is released into the solid . These pressures predominantly concentrate in the centre of contact area or its edges . Lesser and Field  explained that pressure in the contact edge is higher than pressure at the centre (up to 3 times); however, these pressures last for very short duration of time and can be ignored for damage mechanism investigation . Figure 1-3 demonstrates the schematic of a liquid droplet impact onto a solid surface at two different stages, before and after shock envelop detachment. The stress waves, high pressure locations, and the potential cracking sites are highlighted in this schematic.
Figure 1-3: Schematic presentation of a water droplet impingement onto a solid surface: (a) upon impact and before the detachment of disturbed region, (b) after the detachment of disturbed region [3, 23]
In 1928, Cook  posited that the impingement of a liquid jet induces a constant pressure to a solid. He called this pressure “water hammer pressure” and proposed Equation 1-1 to calculate it.
𝑃 = 𝜌0𝐶0𝑉 Equation 1-1
where ρ0 is the liquid density, C0 is the speed of sound in the liquid and V is the impact speed. Equation 1-1 is not accurate to address the impact pressure because it was derived for simplified conditions. Indeed, the peak transient pressure is much higher than the proposed constant value by Cook. Later Heymann  analytically calculated and proposed another equation for the peak
transient pressure generated by the impingement of one droplet, Equation 1-2. It is used in this thesis to address the impact pressure.
𝑃 = 𝜌0𝐶0𝑉[2 + (2𝑘 − 1)𝐶𝑉
0] Equation 1-2
where k is liquid constant. In the case of water erosion, k=2, ρ0=1000kg/m3 and C0=1463m/s. It is worthy to note that the impact pressure is approximately generated over a circle with radius of:
𝑅 = 𝑟 𝑉
Equation 1-3 where r is the radius of the droplet . Due to the compressibility of fluid, the impact pressure in the liquid stay mainly at the centre of impact until the stagnation moment, when the release waves vacate the free surface and the lateral jetting initiates. This is called jetting time and Field  proposed Equation 1-4 to calculate it. He explained that time duration of an impact pressure pulse is around 3 times that of jetting time.
2𝐶02 Equation 1-4
Upon water droplet impact, the disturbance transmits into the solid bythe longitudinal (dilatational) and transverse (distortional) waves traveling at different speeds (C1 and C2). Rayleigh wave is also generated by the droplet impact and it travels on the solid surface with the speed of
CR, shown in Figure 1-4-a [16, 18]. Upon impingement the compressive longitudinal waves expand into the target. Thereby, they interact with microstructural discontinuities and rebound in the form of dilatational tensile waves [16, 18]. The interference of these released and reflective stress waves, shown in Figure 1-4-b, may cause considerable failure especially for a target with nonhomogeneous microstructure .
Figure 1-4: Schematic presentation of: (a) stress waves travelling in the target, (b) reflection and interference of longitudinal and Rayleigh waves [16, 18]
Exerted stresses on the solid during the water erosion can be classified into two main groups. The first group is associated with 'explosive' compressions, which influence the surface for very short time and are referred to as water hammering effect. The second group is a result of the erosive scouring action of the high speed radial outflow jetting . Both groups contribute to the water droplet erosion damage. The physics of liquid/solid impingement becomes more complicated when the repetitive impacts are considered. In this case more parameters, e.g., surface roughness and absorbed energy, involve in the response of target to droplet impacts [26, 27]. Surface roughness varies during the impingements because of localized plastic deformation. Lesser and Field  highlighted that local plastic deformation of solid significantly influences liquid behaviour and its jetting time. Hence, the stress distribution and travelling shock waves differ with surface roughness variation. Once the droplet strikes any asperity on the surface, the high impact pressure coming from the compressed part of the liquid may not be generated. This is due to different deformation behaviour of the liquid. However, hitting a pit may cause even higher impact pressure due to shock wave collisions inside the pit . In addition, the energy of each impingement is partially transferred to the solid surface. This energy may accumulate in the weak points of microstructure, such as grain boundaries, phase interfaces, cracks and porosities, as the vulnerable sites. Once the next droplet strikes these locations, a prompt failure may occur due to the interaction between the new incident impact waves with the reflected waves. This is not the case for the surface impacted by a single isolated droplet.
1.1.2. Damage mechanism of water droplet erosion
A considerable amount of research has been carried out over the last few decades seeking to understand the details of damage caused by water droplet erosion. It is well-known that the erosion damage mechanism is a function of target’s mechanical properties and microstructure, as well as the solid surface conditions (i.e. roughness and presence of stress raisers) [2, 28-31]. To date, it is impossible to predict the water erosion behaviour of a certain material based on the knowledge of its mechanical and physical properties only. Therefore, the response of each material to water droplet impacts and the erosion damage mechanism need to be studied individually. However, some common erosion features found in the early and advanced stages of water droplet erosion are reviewed further.
7 220.127.116.11. Early stages of erosion
In 1985, Field et al.  shed light on the mechanism of erosion damage initiation for ductile targets. They proposed that the repetitive impacts of water droplet on a completely smooth surface cause development of damage in four stages, as demonstrated in Figure 1-5. After initial droplet impacts a shallow depression appears on the surface, shown in Figure 1-5-a. This depression becomes deeper with further impacts. Once the impacting droplet fills the generated depression, the water is thought to be compressed for a longer period of time. This results in greater impact pressure, Figure 1-5-b. The next droplet hitting the deformed location experiences different forms of disturbance, shown in Figure 1-5-c. Here, the angle between the water’s free surface and the water/solid interface is important and if it goes beyond a critical angle, the shock envelope breaks away. The shock waves coming from the walls of deformed area compress the water and make a spear-like central jet . The impact pressure and the strike of this central jet dig the base of depression and generate small central cavity, shown in Figure 1-5-d. This cavity becomes deeper until the air or water, which can be trapped in the pits, play some cushioning role and suppress further deepening .
Figure 1-5: Schematic of erosion damage initiation on a ductile solid surface proposed by Field et al.  Dimples and central depressions are common features reported for the erosion of ductile metals either in the laboratory or in service conditions of turbine blades [16, 32-34]. Other experimental studies have been carried out on a wide range of materials and their response to
droplet impacts were documented in the early stages of erosion [18, 25, 28-30, 35, 36]. Several features of erosion damage at early stages are listed below.
1. Circumferential surface fracture: upon collision the centre of impacted area is under compression. At the same time radial tensile stresses are exerted at the edges of impacted area for short durations. These stresses cause local fractures at the periphery of the droplet on hard and brittle targets, such as plexiglass, shown in Figure 1-6-a . In some cases, an undamaged area in the centre of impact which is surrounded by ring fractures is observed, shown in Figure 1-6-b. Indeed, the fracture of central region is suppressed by induced compressive stresses and only elastic deformation may occur. For hard intermetallic alloys, material loss around the rim of the depression was posited to be the dominant phenomenon ; however, no experimental proof was provided. 2. Depression and localized material flow: the central compressive and subsequent shear
stresses, caused by the water hammering, result in permanent local depression (saucer-shaped), shown in Figure 1-6-c. This is observed mainly for erosion of ductile metals [2, 25, 29, 30] once the dynamic exerted stresses exceed the dynamic yield strength of the solid. In addition to the local penetrations, large amount of micro-plasticity can be observed in the microstructure at high magnification. Slip lines, grain boundaries, and twin boundaries may appear on the surface of depressions [2, 25, 28]. Localized material flow needs to be studied in depth because it facilitates material loss in subsequent stages. Furthermore, the sub-surface flow and subsequent cracking are also observed once droplets impact the ductile targets . In multiphase alloys, the softer phase predominantly shows micro-plasticity. This results in inhomogeneous localized deformation [2, 25, 35].
3. Micro-cracking due to local plastic deformation: surface and sub-surface cracks is often reported as the main erosion features [2, 25, 28-30]. In the case of ductile metals, they mainly initiate due to localized material flow [2, 28-30].
4. Grain boundaries failure: when the size of microstructure constituents is relatively small compared to droplet size, the impacting droplet considerably damage their boundaries. For instance, in erosion of metallic targets grain boundary damage is frequently observed [28, 29, 31, 35]. An eroded surface of aluminium with revealed grain boundaries is shown in Figure 1-6-c. Huang et al.  highlighted that the
rotating of small grains is the main reason for the grain boundary damage in erosion of Ti6Al4V. Different orientation of the grains and subsequent anisotropy were reported as another reason for the grain boundary damage .
5. Circumferential shear fractures: after a few microseconds of impingement and once the shocked envelop in the liquid breaks away, the lateral outflow jets form and hit any surface discontinuity with very high speed. This collision may lead to lateral material flow at the periphery of impacted area or localized fracture of surface asperities such as grinding tracks, elevated grain boundaries, or raised slip bands [25, 31], shown in Figure 1-6-b.
6. Micro-cracking due to stress waves: The travelling stress waves (mainly reflective tensile waves) may generate micro-flaws in the target. These waves interact with microstructural irregularities and initiate cracking . Furthermore, the interference of Rayleigh waves with reflected tensile dilatational waves, shown in Figure 1-4, may cause circumferential fracture on the surface [18, 25, 38], shown in Figure 1-6. This was mainly observed in hard and brittle targets and could be more destructive compared to the other types of failure occurring over the attacked surface area .
Figure 1-6: Eroded surface of: (a) polymethyl methacrylate showing ring fractures , (b) zinc sulphide showing an undamaged area surrounded by annular fractures , (c) aluminum showing the rim of depression and the
revealed grain boundaries 
18.104.22.168. Advanced stages of erosion and material removal
Hancox and Brunton  investigated the response of copper to repetitive droplet impacts. They performed long erosion experiments using low impact speeds (<100m/s). After a few thousand impacts, large number of depressions on the surface of attacked copper were observed. Such localized material flow and surface roughening was put forth as the main cause of material loss initiation . Indeed, peaks of asperities within the roughened surface are broken with the
impact of high speed jets flowing on the surface. Major portion of pitting on the surface of ductile copper was attributed to these impacts . Huang et al.  reported that generation of crack networks and their coalescence is the dominant mechanism of material loss initiation for Ti6Al4V. They highlighted that droplet impacts slightly rotate the grains and cause intergranular cracking, and subsequent micro-pitting. Luiset et al.  reported the grain boundary damage in the initial stages of erosion of stainless steel. They explained that cracks development in the boundaries caused the detachment of grains and the generation of small pits. In several cases, the rupture of grains because of transgranular cracking was also observed. Triple splitting of grains is another mode of material loss which was documented by Kong et al. [36, 40]. The role of grain boundary as an important microstructural defect was elaborated by Hancox and Brunton . They observed that a single crystal of copper shows fewer erosion pits and subsequent slower material loss compared to polycrystalline copper. Generally, erosion progress is associated with abundant cracking. Cracking behaviour is a function of target material properties and the fractography of eroded surface should be carried out for each specific material. However, intergranular cracking for damage initiation and transgranular cracking for the advanced stages were highlighted as the dominant behaviour for erosion of ductile metals [20, 28, 30, 40, 41].
Further droplet impacts on the generated small pits cause a phenomenon called “hydraulic penetration”, which was highlighted as one of the most damaging phenomena in the advanced phases of erosion [3, 20]. Hydraulic penetration was attributed to the formation of spear-like jets inside the cavities. These jets strike the floor of cavities with much larger force compared to the initial droplet impact and bore secondary pits inside the original cavity . Hence, the cavities enlarge and merge together with further impingements. The coalescence of enlarged cavities causes detachment of large fragments and the generation of deep craters. In these stages water hammering, lateral jetting, and water penetration contribute to the erosion damage progress [2, 3, 20]. Droplet impacts on the deep craters result in inhomogeneous stress distribution and formation of different types of pits on the bottom and the sidewall of craters. For instance, generation of narrow and undercutting pits, called tunnels and sub-tunnels, were documented in the case of Ti6Al4V erosion . Their generation roughens the surface along the edges of erosion craters. The vulnerable sites over the roughened surface will be broken with oncoming droplet impacts. Their fracture smooths the eroded surface, which was called water smoothing [41, 42].
11 1.1.3. Parameters affecting liquid droplet erosion
Liquid droplet erosion is a complex phenomenon which is a function of numerous parameters. They are classified into two main categories [2, 43]. The first group comprises liquid and solid properties including their densities, liquid viscoelasticity behaviour, and mechanical properties of solid target. The second group includes the impingement parameters such as impact speed, impact angle, droplet size, and its shape, which are mainly the interest of this thesis and thus reviewed further.
22.214.171.124. Impact speed
Water droplet erosion as repetitive impact wear is a function of impact speed because the induced pressure and kinetic energy of each impact are influenced by the velocity. Coulon  described that impact speed is significantly important since it changes the nature of damage (chemical or mechanical). Based on the impact speed, he divided the damage caused by liquid/solid interaction into four groups; corrosion, corrosion-erosion, erosion-corrosion, and erosion . He explained that above a critical impact speed, no chemical degradation (corrosion) can be seen for liquid/solid interaction and there is only mechanical degradation (erosion). On the other hand, several experimental investigations showed that below a critical impact speed no mechanical degradation occurs [7, 45, 46]. However, Heymann  questioned this point and explained that mechanical damage happens at all speeds; however, it needs very long exposure to erosion. Furthermore, the relation between impact velocity and erosion rate, the most important indicator of erosion damage, was of great interest in previous works. Different functional forms were used to fit the experimental data for this relation [7, 8, 45-48] and they are reviewed in chapter 2.
126.96.36.199. Impact angle
In service conditions, blade twisting and air turbulence in the chamber result in different impact angles along the turbine blades. Therefore, the influence of impact angle on erosion behaviour was studied in the literature and it was mainly described by its effect on the impact speed [2, 32, 49]. Water erosion is a strong function of normal impact velocity and this velocity varies with changing the impact angle. The influence of impact angle was explored during the incubation period of erosion and before the formation of craters, because the crater formation leads
to lose of control of the impact angle . Heymann  explained that even during the incubation period studying the influence of impact angle is challenging because of the surface roughness variation. This implies that the impact angle affects only very early stages of erosion and some researchers such as Lee et al.  claimed that this effect could be neglected. However, Ahmad  recently reported a notable influence of impact angle on water erosion, shown in Figure 1-7. The maximum erosion damage, cumulative volume loss after 50h, occurred at impact angle of 90° which is associated with the maximum normal component of impact velocity. In the case of solid particle erosion, the impact angle associated with the maximum damage depends on the target mechanical properties. It is 22.5° for ductile materials and 90° for brittle materials .
Figure 1-7: Normalized material loss of stainless steel eroded at different impact angles 
188.8.131.52. Droplet size
Another parameter affecting water erosion damage is the size of impacting droplets. The droplet size influences the area exposed to the impacts, time duration of each impact pulse, distribution of impact pressure, and the transferred kinetic energy [2, 49, 51]. The general trend is that increasing droplet size accelerates the erosion damage. Heymann  explained that using same volume of water, larger droplets cause more and faster damage. Although the target is impacted by greater number of smaller droplets, these impacts are not as destructive as large droplet impacts. This was explained by fatigue-like mechanism of erosion damage and detrimental kinetic energy of water droplets [2, 27]. Besides, it was claimed that the damage caused by water erosion is a function of droplet radius at the contact area and not its mass . It denotes that the droplet shape also affects the erosion damage. Hence, the radius of flattened area must be taken as the influencing radii for a deformed droplet in the contact region. It has been argued that a small
flattened droplet behaves similar to a larger sphere droplet [18, 52]. This would be correct for the stress distribution; however, it can be questioned in term of transformed kinetic energy. This energy is a direct function of droplet mass/volume and the difference in amounts of kinetic energy for a small flattened droplet versus a large sphere droplet is significant.
1.1.4. Time dependence of water droplet erosion
Erosion is a progressive and time-dependent mechanical damage. As explained earlier, the localized plastic deformation, micro-cracking, and local fractures cause material removal during erosion. Time dependence of cumulative material loss has a non-linear nature, similar to what was observed for the cavitation erosion . Figure 1-8 demonstrates different forms of erosion graphs, cumulative material loss versus cumulative exposure duration. Curve A is the typical S-shaped graph, which is seen for erosion of bulk materials. Curve B could be seen when the erosion conditions, i.e. impact speed and droplet size, are severe for the target. Curves C and D are anomalous for the erosion damage and therefore cannot be accepted. It is worthy to note that the erosion results of surface treated coupons do not necessarily fit in the aforementioned graphs and their behaviour depends on surface structure and microstructure.
Figure 1-8: Different forms of erosion graphs 
Typical S-shaped erosion graph was divided by Heymann [2, 53] into five distinct stages, shown in Figure 1-9-a.
A. Incubation stage: At the beginning of erosion, droplet impacts mainly cause local material flow and micro-cracking; however, no material loss or a little can be detected, as can be seen in curve A of Fig 1-8. This stage may be very short and not observed in the case of
severe erosion conditions, when initial droplet impacts cause detectable material loss. This is demonstrated in curve B in Figure 1-8.
B. Acceleration stage: Immediately after the initiation of micro-pitting, greater material removals could be seen with further droplet impacts. In this stage, the erosion rate grows rapidly and reaches its maximum value, as shown in Figure 1-9. This period is associated with coalescence of the generated pits and noticeable increase in the size of the crater. C. Maximum erosion rate stage: In this stage the material loss rate remains constant or
nearly so, resembling the maximum erosion rate. The formed craters in this period of erosion become deeper and larger.
D. Deceleration or attenuation stage: Once erosion craters reach a certain depth, erosion rate decreases notably (25 to 50% of maximum erosion rate). It was attributed to the very high roughness of eroded surface (generated peaks and pits), which changes the stress distribution. Also, some water which is trapped in the crater may cushion the impact and decelerate the erosion damage.
E. Terminal steady state stage: This is the last stage of erosion evolution, when the material loss rate becomes again constant or nearly so. This stage was not captured in water droplet erosion of brittle materials.
Figure 1-9: (a) Typical water droplet erosion and (b) erosion rate graphs showing five different stages 
1.1.5. Representation of water droplet erosion results
Erosion results are conventionally represented using the cumulative materials loss (vertical axis) as a function of cumulative erosion exposure duration (horizontal axis). They are referred to
as water droplet erosion graphs. In addition, erosion rate graphs are also considered in the literature, shown in Figure 1-9-b. They are beneficial to track down the erosion performance during the whole experiment. In open literature, erosion rate graphs are mainly plotted with the instantaneous erosion rates, which are the slopes of the lines connecting two consecutive points on the erosion graphs [2, 8, 46, 53, 55]. However, Rao & Young  proposed to use the cumulative erosion rates, which is the slope of the lines connecting the origin to each point on the erosion graphs, in order to diminish possible bios and noises. The cumulative erosion rate is not a popular idea in the literature; however, it was used by Ahmad et al. [8, 51] to find Cumulative Erosion Resistance (CER). CER is the reciprocal of cumulative erosion rate at the end of experiment.
The erosion graphs are represented in the literature with different parameters trying to capture the maximum amount of information in these graphs [2, 7, 8, 35, 41, 46, 48, 51, 57, 58]. For the vertical axis, either mass loss or volume loss were used [7, 8, 35, 41, 46, 58]. However, various parameters were used to represent the erosion exposure duration. Erosion time [8, 59-61], number of cycle [41, 51, 62], droplet/jet impact number [46, 63], droplet/jet energy  and volume of impacting droplets  were used to represent the erosion exposure. This makes comparison of the previous results impossible. ASTM standard G73  describes the basic approach for erosion investigation and guidelines for results representation, which are used in this thesis.
In order to plot the erosion graphs, the experiments are interrupted at different time intervals to weigh the coupons and record the mass loss. This mass loss is converted to the volume loss knowing the density of tested coupons. Recording the cumulative mass loss at different time intervals reveals the points constructing the erosion graph, shown in Figure 1-10-a. ASTM standard G73 recommends to use volume loss (vertical axis) versus volume of water droplets impacting the surface (horizontal axis) for erosion graphs. This approach results in the dimensionless slope for the erosion graph, which would be necessary for the comparative studies. However, exact volume of impacting water was not known in most of the previous studies. Using the erosion graph, three important erosion indicators could be extracted, incubation period (H0), maximum erosion rate (ERmax), and final erosion rate (ERfinal), as shown in Figure 1-10-b [2, 54]. The first two can be found for all materials; however, the last one may not be revealed during the erosion of brittle materials . Indeed, there is a relatively large variation for the final erosion rate
of such materials because of the brittle fractures leading to the detachment of relatively large fragments [25, 64]. In addition, very long experiments are required to reach the final steady state stage for the erosion resistant materials. In this thesis, incubation period (H0) and maximum erosion rate (ERmax) are used to represent the erosion performances. ERmax is extracted by fitting the best line through the points in stage C, shown in Figure 1-10-a. The slope of this line is taken as ERmax. In addition, the intersection of this line with erosion exposure axis is taken as the incubation period (H0), as shown in Figure 1-10-b . Since the surface treated coupons do not usually show the typical S-shaped erosion graph, using the mentioned indicators for them is challenging. Therefore, cumulative erosion resistance (CER) are mainly used in this work for comparative investigations. CER is defined as the ratio of total volume of impacting water to total volume loss of the target. This indicator reflects the total resistance of the material to water droplet erosion. It is noteworthy that the erosion resistance, which is used further in the thesis, is inversely proportional to the erosion rate.
Figure 1-10: (a) Typical S-shaped erosion graph plotted through experimental points, (b) extracting the erosion indicators from material loss graphs [2, 54]
ASTM standard G73 describes a certain procedure to study the influence of impingement parameters (e.g., impact speed) on the erosion behaviour. Indeed, the results must be expressed using physically meaningful variables, which are dimensionless. Hence, the incubation period (H0) is represented using specific number of impacts. Also, the rationalized erosion rates (RER) are used. These parameters are explained in detail in chapter 2. Furthermore, using a reference coupon in each erosion experiment is strongly recommended in ASTM standard G73. This approach allows to represent the erosion behaviour of each coupon with respect to that of the reference pair.
This is beneficial in order to detect small changes in water erosion performances. In this work, Ti6Al4V is used as the reference coupon in erosion experiments.
In summary, the erosion and erosion rate (instantaneous rate) graphs (Figure 1-9) are plotted as the basic erosion results. From these graphs, erosion indicators are extracted and the ones reported in this thesis are as follows: Incubation period in terms of either volume of impacting water or specific number of impacts (H0); Maximum erosion rate (ERmax or RERmax); and Cumulative erosion resistance (CER) of each sample normalized to CER of Ti6Al4V pair. More details on erosion experiments could be found in Appendix.
1.2. Promising water droplet erosion resistant materials and surface treatments
Erosion resistance have been widely correlated to the mechanical properties of the target such as yield strength and hardness, ultimate resilience (Su/2E, where Su is ultimate strength and E is modulus of elasticity), true stress at fracture, strain energy to fracture, and work hardening rate [2, 8, 12, 65, 66]. Amongst these parameters, yield strength and modulus of elasticity were introduced as the most important ones by Heymann . The material strength is the most corresponding index to erosion performance. Usually the higher the mechanical strength, the more the erosion resistance . The mechanical strength is more important in the surface of target and it can be addressed by hardness. In order to enhance WDE of turbine blades, either a new stronger alloy should be used or the surface of currently used alloy (Ti6Al4V) must be hardened. Based on the high strength of TiAl alloy and its superior cavitation erosion resistance [67-69], it would be a promising water droplet erosion resistant material especially because it is even lighter than Ti alloys. Therefore, its WDE performance and damage mechanism are comprehensively investigated in chapters 2 and 3.
Surface of Ti6Al4V is being modified using different techniques. They can be classified into four main groups: thermal treatments; thermochemical treatments; deposition of thin films; and fabrication of thick coatings . Surface treated samples using the mentioned techniques are schematically presented in Figure 1-11. Applying a thermal surface treatment such as laser hardening hardens the surface due to phase transformation and microstructure refinement. The main challenge for this process is controlling the formation of micro-cracks due to rapid solidification . These micro-cracks would be detrimental in erosion applications. Thermochemical treatments harden the surface by making two main layers on the sample. The first
one is compound layer, which is hard and brittle ceramic film. The level of porosity and adhesion strength to the sample are the main parameters determining the mechanical stability of compound layer. Beneath this layer, there is a diffusion layer which is hardened by the formation of interstitial solid solutions [70, 72]. Solid solution strengthening increases the hardness without adding an interfaces, which is suitable for erosion applications. Thermochemical treatments require high temperature and it may change the microstructure of base material. To avoid this, hard and thin films at relatively low temperatures are fabricated on the substrate using vapour deposition methods such as Cathodic Arc Physical Vapor Deposition (CAPVD). The main issues for vapour deposited films are the formation of micro-cracks and micro-pores within the films, their residual stresses, and their adhesion to the substrate . These films are vulnerable when they are subjected to the harsh mechanical loading. The last technique is thermal spray coating, which is used to fabricate thick layers on the surface by spraying various powders. . The main issues for sprayed coatings are their porosity, adhesion of splat boundaries and the quality of coating/substrate interface . Such microstructural defects would be detrimental for WDE application because they facilitate the cracking upon droplet impacts and stress wave propagation.
Figure 1-11: Different surface treatments of titanium alloys: (a) thermal treatments, (b) thermochemical treatments, (c) thin film deposition, (d) thermal spray coating
Water droplet erosion performance of surface treated Ti6Al4V have been rarely investigated. However, their cavitation erosion behaviour have been well studied in the literature [74-77]. The nature of cavitation erosion damage and water erosion damage is similar because in both cases hydrodynamic forces are exerted on the sample. Therefore, available literature for both cavitation and water erosion performance of surface treated Ti6Al4V and stainless steel are reviewed. Figure 1-12 demonstrates the erosion resistance of bulk TiAl and surface treated coupons normalized to their reference material (i.e. Ti6Al4V or stainless steel). Herein, the erosion
resistance were taken from different articles. In some of them, only the level of improvement at the end of experiment is given without clear definition for the considered erosion indicators [67, 74]. In the other ones, the erosion graphs are provided [76, 78-80]; however, there are different scales for the erosion graphs and no standard indicator is considered. In order to have relatively fair comparison, CER was derived from erosion graphs and then normalized by CER of reference material in that article. It is noteworthy that this graph is not a very accurate comparison because of different reference materials, different experimental setups, and different erosion conditions used in the previous studies. However, it provides general ideas about the potential of different surface engineering techniques or materials to combat erosion.
Nitriding is the most common thermochemical treatment applied on titanium alloys. Nitrided Ti6Al4V demonstrates superior erosion resistance almost at all of the previous studies, shown in the second column of Figure 1-12. Erosion performance of nitrided Ti6Al4V depends on the utilized nitriding parameters which are reviewed in chapter 4. Sprayed cermet coatings are found resistant to erosion; however, large variation can be seen for their performance [48, 62, 79]. In a few cases, they showed even worse performance compared to the substrate. The reasons for such variation are explained in chapter 5. Laser hardening enhanced the erosion resistance of Ti6Al4V and stainless steel in all previous investigations. Unlike laser hardened samples, vapour deposited hard films do not always show superior erosion resistance. The last column in Figure 1-12 indicates that the ratio of erosion resistance of coated sample to that of reference material is between 0.4 and 11. This ratio is highly dependent to the mechanical stability of deposited thin films, their thickness, and erosion severity. The more aggressive the erosion conditions, the less the erosion resistance of vapour deposited samples.
Figure 1-12: Cumulative erosion resistance of TiAl intermetallic and surface treated Ti6Al4V normalized to that of reference material [48, 61, 67, 68, 74-76, 78-81]
The main objective of this research is to improve water droplet erosion resistance of gas turbine compressor blades. Two approaches are used to tackle this objective: (1) proposing an erosion resistant alloy which can be potentially used for the compressor blade; (2) enhancing the erosion resistance of Ti6Al4V using two different surface treatments. To achieve the main objective, the sub-objectives are defined as follow:
- Studying water droplet erosion of nearly fully lamellar TiAl alloy
o Investigating erosion performance of TiAl compared with Ti6Al4V at different impact velocities and droplet sizes
o Understanding the erosion damage mechanism of TiAl alloy at different phases of erosion including the incubation, material loss initiation and advanced stages
- Studying the influence of gas nitriding treatment on water droplet erosion behaviour of Ti6Al4V
o Investigating the erosion performance of Ti6Al4V which are nitrided at different conditions in comparison with non-treated Ti6Al4V
o Understanding the erosion damage mechanism of gas nitrided Ti6Al4V
- Exploring the potential of WC-Co coating sprayed by HVOF technique to combat water
droplet erosion damage
o Investigating the erosion performance of WC-Co coatings sprayed at different conditions in comparison with Ti6Al4V
1.4. Thesis layout
This section outlines the format of the current manuscript-based thesis. This document consists of six chapters. Chapter 1 gives an introduction about water droplet erosion. The physic of solid/liquid impact are briefly described, the erosion damage mechanism is reviewed, and the common methods to represent the erosion results are highlighted. Afterward, the objectives of this thesis are presented. In chapter 2, the erosion performance of TiAl is investigated compared with Ti6Al4V. The influences of impact velocity and droplet size are examined on the erosion behaviour of these structural alloys. In addition, the critical impact speed or damage threshold (VC) for water droplet erosion of TiAl is determined. In this chapter, it is verified that water droplet erosion resistance of TiAl is superior to that of Ti6Al4V at all erosion conditions. Hence, chapter 3 presents in-depth investigation of WDE damage mechanism for nearly fully lamellar TiAl alloy. The eroded coupons at different phases: incubation, material loss initiation, maximum erosion rate and advanced stages of erosion are characterized. In order to address the second approach mentioned in the objectives, chapter 4 is dedicated to the influence of gas nitriding on water erosion behaviour of Ti6Al4V. Ti6Al4V specimens which were nitrided at two different temperatures (900 and 1050°C) for 5 and 10 hours are characterized. Their erosion behaviour in comparison with as-received and annealed Ti6Al4V are examined at two different impact speeds. Afterwards, erosion damage mechanism of the nitrided coupons is described. In chapter 5, potential of WC-Co thermal sprayed coatings are examined to combat water droplet erosion. Two different WC-Co powders were sprayed using HVOF technique, and two relatively thick cermet coatings with different microstructures were obtained. Their erosion performance in comparison with the as-received Ti6Al4V are explored at three different impact speeds (i.e. 250, 300, and 350m/s). Afterward, the erosion damage mechanism of coatings with splat microstructure are explained. Chapter 6 summarizes the findings in this research and presents the conclusions, contributions, and recommendations for future work. At the end of each manuscript, a short text is added to connect the chapters and ensure the coherency of the thesis.
Figure 1-13: Flowchart of the thesis